EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING

 Jeffery Sparks
 8 months ago
 Views:
Transcription
1 Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1, Samar Chandra Mondal 2, Susenjit Sarkar 3 1 Jadavpur University, Faculty of Engineering Technology, Department of Mechanical Engineering, Kolkata, India, 2 Jadavpur University, Faculty of Engineering Technology, Department of Mechanical Engineering, Kolkata, India 3 Jadavpur University, Faculty of Engineering Technology, Department of Mechanical Engineering, Kolkata, India Abstract: Analytical formulation and solution of stress analysis of composite plate subjected to thermo mechanical loading for various ply orientation and thickness of lamina are studied. The main aim of the paper is to investigate how mechanical and thermo mechanical loading would affect the stress ratio and stress distribution of composite plate. The plate is composed of layers of glassepoxy composite and the orientation of the layers is assumed to be antisymmetric about the neutral axis of the laminate. The plate is subjected to a combined mechanical loading of tensile force and moment along x direction. The thermo mechanical stress is calculated for different ply orientation and thickness ratio, subjected to a temperature change and mechanical loading. The effect of number of lamina and varying thickness of laminate on the stress ratio and stress distribution is studied. The results in this paper are obtained by use of MATLAB Programming and by Finite element software ANSYS 14. Results obtained from both the methods are compared. Such type of loading finds wide application in aircraft flying at high altitude, marine application, medical devices etc. KEYWORDS: Ply orientation, classical lamination theory, thermo mechanical, laminate. 1. Introduction Composite material is a structure that is composed of two or more material combined at a macroscopic label and are not soluble to each other, in such a way that one phase is called reinforcing phase and the other phase in which it is embedded is called matrix. Reinforcing phase may be in the form of fiber, flakes, particles etc. Laminated composite find wide application in aerospace, marine, medical, automobile etc. Industries owing to their advantages of high strength, fatigue life, stiffness, temperaturedependent behavior, corrosion resistance, thermal insulation, wear resistance, thermal conductivity, attractiveness, acoustical insulation and low weight. The increase in the strength, stiffness and reduction in weight of engineering structure can be achieved by using composite material. Further reduction can be achieved by using optimum ply orientation, thickness or stacking sequence. Most of the research is focused on design of composite structure for optimum ply orientation and stacking sequence. L. W.Chen & L. Y.Chen[1] studied the effect of thermal stress in composite plate by using finite element method. Onur Sayman [2] studied an elastic plastic type of thermal stress analysis which was carried on metal matrix composite beams of fiber reinforced of steel and metal matrix of aluminum. R. Özcan [3] explained through his paper about residual stress analysis of a thermoplastic laminated composite plate for an in plane loading. Frank R. Jones, Fangming Zhao [4] investigated the effects of thermal stresses developed on the stress transformation between resin and short fiber using the method of photo elasticity. Wu and DOI: /scjme2171, Print ISSN , Online ISSN SjF STU Bratislava
2 Tauchert [4,5] developed a model to obtain thermal stresses and deformations in anti symmetric angle ply and cross ply laminates and symmetric laminates. Noor and Burton [6] obtained solutions for the bending, buckling and vibration of antisymmetrically laminated rectangular plates, periodic in the inplane directions. Savithri and Varadan [7] studied plates under uniformly distributed and concentrated loads. P. Vidal et al. [8] presented the thermomechanical analysis of bidimensional laminated beams by using a variables separation method. Thermal and mechanical responses are assessed by comparing with other approaches available in literature, exact solutions and 2D finite element computation. Zineb et al. [9] study the influence of varying thickness glass epoxy composite plate under the pure bending moment. Joshi & Biggers [1] determine the optimal thickness distribution over the plate, for which the thickness distributions that maximize the buckling load are determined. Javadi et al. [11] formulate a three dimensional solutions for contact area in laminated composite pinned joints with symmetric and nonsymmetric stacking sequences. Kormaníková, E. [12] studied an optimal design of laminate circular cylindrical. Choudhary S, et al. [13] formulate a simple higher order theory for dynamic analysis of composite plate. Most of the research paper focuses on the optimum design of composite plate by optimizing thickness for bending, buckling, vibration or thermal load using finite element method or variable separation method. Ply orientation is a very important parameter which effects the stress distribution in composite plate. Research paper on the study of the effect of ply orientation on stress analysis of composite plate under thermo mechanical load is rare. Thermo mechanical stress can be calculated by classical laminate theory, the first order shear deformation theory, higher order theories and finite element method. In this paper classical laminate theory is used to compute the stresses in a four layered anti symmetric composite plate under different ply orientation and loading conditions. Thermo mechanical stress is determined by superposing the stress generated for the mechanical and thermal loading condition. The study is carried out for angle ply orientation varied from degree to 9 degree. The effect of no. of lamina and varying thickness ratio on the stress ratio and stress distribution of composite plate is studied. This paper determines the stress ratio for different orientation of the lamina to check which stacking sequence would give the lowest ratio. The stacking sequence of the laminate with the lowest stress ratio is likely of an optimized type. 2. Analysis of composite plate A laminate is a collection of lamina arranged in a specified manner. Adjacent lamina may be of the same or different materials and their fiber orientations with respect to a reference axis (by convention, the xaxis) may be arbitrary. Classical lamination theory (CLT) is applicable to orthotropic continuous fiber laminated composites only. the classical lamination theory is only valid for thin laminates (span a and b > 1 thinckness t ) with small displacement w in the transverse direction (w << t) [ IIT lecture notes] 2.1. Assumption of Classical lamination theory (CLT) The assumptions of classical lamination theory are stated as [14]: 1. Each layer of the laminate is quasihomogeneous and orthotropic. 2. The laminate is thin compared to the lateral dimensions and is loaded in its plane. 3. State of stress is plane stress. 4. All displacements are small compared to the laminate thickness. 5. Displacements are continuous throughout the laminate SjF STU Bratislava Volume 67, No. 1 (217)
3 6. Straight lines normal to the middle surface remain straight and normal to that surface after deformation. 7. Transverse normal strain ε z is negligible compared to the inplane strains ε x and ε y. 8. Straindisplacement and stressstrain relations are linear. 2.2 Stress analysis of lamina A lamina is a thin layer of a composite material that is generally of a thickness on the order of.5 in. (.125 mm). A laminate is constructed by stacking a number of such lamina in the direction of the lamina thickness. The constitutive equations for a general linear elastic solid relate the stress and strain tensors through the expression: σ ij = C ijkl ε kl, ε ij = S ijkl σ kl (i, j, k, l = 1,2,3) (1) Where C ijkl = stiffness components, S ijkl = compliance components. Fiber reinforced composite materials are considered to have orthotropic elasticity because these materials possess three mutually perpendicular planes of the elastic symmetry. For a unidirectional reinforced lamina in the 12 plane as shown in Figure, a plane stress state is defined by: σ 3 =, τ 23 =, τ 31 = σ 1, σ 2, τ 12 Moreover the stress strains relations in 12 planes: where Q 11 = E 1 1 ν 12 ν 21 σ 1 Q 11 Q 12 Q 11 ε 1 [ σ 2 ] = [ Q 12 Q 22 ] [ ε 2 ] (2) σ 3 Q 66 γ 12,Q 22 = E 2 1 ν 12 ν 21 Strain stress relation is obtained as:, Q 12 = Stress strain relation in x y coordinate system: ν 12 E 2 1 ν 12 ν 21, Q 66 = G 12, ν 12 E 1 = ν 21 E 2 [ε] = [Q] 1 [σ] (3) σ x Q 11 Q 12 Q 16 ε x [ σ y ] = [ Q 12 Q 22 Q 26 ] [ ε y ] where [Q ] = [T] 1 [Q][R][T][R] 1 (4) τ xy γ xy Q 16 Q 26 Q Stress analysis in laminate C 2 S 2 2CS 1 T = [ S 2 C 2 2CS ] and R = [ 1 ], SC SC C 2 S 2 2 where C = cos θ, S = sin θ Determination of laminate stiffness [A B D] matrix Consider a laminate made of n plies shown in Figure 4.6. Each ply has a thickness of tk. Then n the thickness of the laminate h is h = k=1 t k Then, the location of the mid plane is h/2 from the top or the bottom surface of the laminate. The zcoordinate of each ply k surface (top and bottom) is given by: k 1 h k 1 = h 2 + t 1 (top surface), h k 1 = h 2 + t Volume 67, No. 1, (217) 217 SjF STU Bratislava 7 k 1 (bottom surface) (5)
4 (a) (b) Fig. 1 (a) Rotation of Principle material axis from reference xy axis, (b) location of plies in laminate [15] (a) (b) Fig. 2 Composite plate subjected to (a) Normal force/ length, (b) Bending moment / length [15] (a) (b) Fig. 3 Composite plate subjected to (a) combined mechanical load (normal force and bending moment), (b) Thermo mechanical load Force per unit length (N) and the bending moment per unit length(m) of a laminate are given as: N x A 11 A 12 A 16 [ N y ] = [ A 12 A 22 A 26 ] [ N xy A 16 A 26 A 66 ε x ε y γ xy B 11 B 12 B 16 ] + [ B 12 B 22 B 26 ] [ B 16 B 26 B 66 k x k y ] (6) k xy SjF STU Bratislava Volume 67, No. 1 (217)
5 M x B 11 B 12 B 16 [ M y ] = [ B 12 B 22 B 26 ] [ M xy B 16 B 26 B 66 ε x ε y γ xy D 11 D 12 D 16 ] + [ D 12 D 16 D 22 D 26 D 26 ] [ D 66 N x, N y, = normal force per unit length, N xy = shear force per unit length, k x k y ] (7) k xy M x, M y, = Bending moment per unit length, M xy = Twisting moments per unit length ε = midplane strain of laminate in xy coordinate and k =laminate curvature. Combining the above two matrix as: { N B } = [A M B D ] [ε k ] (8) n A ij (extensional stiffness matrix) = k=1 [Q ] ij k (h k h k 1 ), i = 1,2,6, j= 1,2,6 B ij (extension bending coupling matrix) = 1 n [Q ] 2 ij k (h 2 2 k=1 k h k 1 ), i = 1,2,6, j= 1,2,6 D ij (bending stiffness matrix) = 1 n [Q ] 3 ij k (h 3 3 k=1 k h k 1 ), = 1,2,6, j= 1,2, Determination of stress of laminate The mid plane strain and curvature can be determined from ABD matrix as: ε k = A B N B D 1 [ M ] (9) Stresses of laminate in the k th lamina as: Strain of laminate in the k th lamina as: 2.4 Thermo mechanical stresses [σ] k = [Q ] k [ε ] + h[q ] k [k] (1) [ε] k = [ε ] + h[k] (11) Thermal stresses are developed due to cooling down or heating from processing temperatures to operating temperatures different from processing temperatures. Each ply in a laminate gets stressed by the deformation differences of adjacent lamina. The mechanical strains developed by thermal loads are: [ε M ] = [ε] [ε T ] where [ε] = [ε ] + z[k] (12) The thermal stresses are given by: Mid plane strain and curvature is calculated by: where [σ T ] = [Q ][ε M ] (13) [ NT M T] = [A B B [N T n ] = T [Q ] ij [α] k k (h k h k 1 ) D ] [ε k ] (14) k=1, n [M T ] = 1 2 T [Q ] ij [α] k k (h 2 2 k h k 1 ) k=1 Volume 67, No. 1, (217) 217 SjF STU Bratislava 9 (15)
6 Thus, if both mechanical and thermal loads are applied, then superpose the mechanical loads to the fictitious thermal loads to find the plybyply stresses and strains in the laminate or separately apply the mechanical and thermal loads and then add the resulting stresses and strains from the solution of the two problems. Stress ratio can be calculated as: 3. Problem formulation Stress ratio () = Maximum stress Minimum stress A composite plate made up of four layers glass epoxy material subjected to combined loading condition (shown in fig) is considered for study. The layers are arranged anti symmetrically [+ α + α α]. Stresses developed in the composite plate for different ply orientation (  9 ) are studied for loading condition: combined load of normal force and bending moment in x direction. (N x = 1 N m, M x = 4 N m). The effect of lamination angle on the stress distribution of composite plate is analyzed for different length to thickness ratio (a/h) of composite plate. Stress ratio is computed for a/h ratio of 5, 1 and 2. Classical lamination theory is used to model the stress analysis of composite plate. From this analysis the optimum lamination angle corresponding to minimum stress ratio can be obtained. The properties of glass epoxy composite material are shown in the table. The entire ply is of equal thickness. Fiber volume fraction Table 1: Properties of Glass epoxy composite Longitudinal Transverse Shear Modulus modulus of modulus of (G12) elasticity (E1) elasticity (E2) 6% 38.6 GPa 8.27 GPa 4.14 GPa.3 Poisson s ratio (ν 12 ) (16) A. Steps to analyze composite plate a) Determine the reduced stiffness matrix [Q] for each ply (eq. 2) using the properties of composite material (table1) b) Determine the transformed reduced stiffness matrix [Q ] for each ply (eq. 2) using [Q] and angle of orientation. c) Determine the coordinate of the top and bottom surface of the laminate (eq.5) d) Determine the laminate stiffness ABD matrix (eq. 8) using [Q ] and coordinate of the laminate. e) Determine the mid plane strain and curvature by substituting the value of ABD matrix and applied force and moment (eq. 9). f) Determine the global stress and strain in each ply (eq.1, eq. 11) using mid plane strain and curvature and location of each ply. 4. Result and Discussion The stress analysis in composite plate subjected to thermo mechanical load for different layer orientation, thickness and number of lamina is computed by using Classical lamination theory method (CLT). CLT is solved by developing MATLAB program and by using ANSYS software. The lamina is arranged anti symmetrically in the laminate. The lamination angle is SjF STU Bratislava Volume 67, No. 1 (217)
7 varied from to 9. Since magnitude of stress at and 9 lamination angle are almost same. The influence of lamination angle and thickness on the stress distribution in composite plate subjected to thermal load only and combined normal force and bending moment in x direction is also studied. Minimum stress ratio for mechanical load and thermo mechanical load is obtained at lamination angle [+3] and [+6] respectively (table 2 & 3). Whereas for thermal load stress ratio remain constant for different lamination angle. Therefore the optimum lamination angle for combined mechanical load is [+3] and for thermo mechanical load is [+ 6]. Table 2 and 3 shows the comparison of stress ratio () obtained from Classical Lamination Theory (CLT) with FEA (ANSYS) respectively. Both the result shows good agreement with each other with minor percentage error (3% 5%). Fig 4, 5 and 6 shows the effect of lamination angle on stress distribution in composite plate subjected to mechanical load, thermal load and thermo mechanical load respectively. Optimum lamination angle for mechanical load is [+3], [+45] and [+35] for stress along x axis, y axis and shear stress respectively. Optimum lamination angle for thermal load and thermo mechanical load is [+3], [+6] and [+45] for stress along x axis, y axis and shear stress respectively. And all the stresses are zero for and 9 lamination angle. Fig 7, 8 and 9 shows the variation of stress with laminate thickness ( z h ) for lamination angle [+]as,[+9]as, [+ 3]as, [+6]as and [+ 45]as for mechanical load, thermal load and thermo mechanical load respectively. Fig1 shows that stress ratio decreases with the increase of a h ratio for different lamination angle and stress ratio for mechanical load is greater than that of thermo mechanical load. Stress ratio () for thermal load is constant. Fig 11 shows that optimum stress ratio is obtained at lamination angle of [+3] for mechanical load and [+6] for thermo mechanical load for different a/h ratio. Fig 12 shows the variation of stress ratio with a/h ratio for different lamination angle for mechanical and thermo mechanical load. Fig 13 shows that stress ratio decreases with the increase of the number of lamina. Table 2 Comparison of stress ratio () obtained from Classical Lamination Theory with FEA (ANSYS) for mechanical load. MECHANICAL LOAD STRESS RATIO CLT ANSYS LAMINA a/h STACKING SEQUENCE STACKING SEQUENCE []s [3]s [45]s [6]s [9]s []s [3]s [45]s [6]s [9]s Volume 67, No. 1, (217) 217 SjF STU Bratislava 11
8 SHEAR STRESS XY () STRESS X() STRESS Y() Table 3 Comparison of stress ratio () obtained from Classical Lamination Theory with FEA (ANSYS) for thermo mechanical load. THERMO MECHANICAL LOAD STRESS RATIO CLT ANSYS LAMINA a/h STACKING SEQUENCE STACKING SEQUENCE []s [3]s [45]s [6]s [9]s []s [3]s [45]s [6]s [9]s T1 B1 T2 B2 T3 B3 T4 B T1 B1 T2 B2 T3 B3 T4 B LAMINATION ANGLE(DEG) LAMINATION ANGLE(DEG) List of symbols used σ Stress G Shear modulus ε Strain θ Poisson s ratio θ Lamination angle(deg) T1 Top of layer 1 γ Shear strain at plane B1 Bottom of layer1 τ Shear stress at plane T2 Top of layer 2 E Young s Modulus B2 Bottom of layer 2 h Total laminate thickness T3 Top of layer 3 z thickness B3 Bottom of layer3 a Plate length T4 Top of layer T1 B1 T2 B2 T3 B3 T4 B LAMINATION ANGLE (DEG) Fig. 4 Composite plate subjected to combined mechanical load (N x = 1 N m, M x = 4 N m and a h = 5) a) stress in x direction b) stress in y direction c) Shear stress XY for different lamination angle SjF STU Bratislava Volume 67, No. 1 (217)
9 SHEAR STRESS XY, STRESS X, STRESS Y, LAMINATION ANGLE (DEGREE) T1 B1 T2 B2 T3 B3 T4 B LAMINATION ANGLE(DEGREE) T1 B1 T2 B2 T3 B3 T4 B T1 B1 T2 B2 T3 B3 T4 B LAMINATION ANGLE(DEGREE) Fig. 5 Composite plate subjected to thermal load ( T = 75 ) a) stress in x direction b) stress in y direction c) Shear stress XY for different lamination angle. Volume 67, No. 1, (217) 217 SjF STU Bratislava 13
10 SHEAR STRESS XY, STRESS X, STRESS Y, T1 B1 T2 B2 T3 B3 T4 B T1 B1 T2 B2 T3 B3 T4 B LAMINATION ANGLE (DEGREE) LAMINATION ANGLE(DEGREE) T1 B1 T2 B2 T3 B3 T4 B LAMINATION ANGLE(DEGREE) Fig. 6 Composite plate subjected to Thermo mechanical load (N x = 1 N m, M x = 4 N m, T = 75 and a h = 5) a) stress in x direction b) stress in y direction c) Shear stress XY for different lamination angle SjF STU Bratislava Volume 67, No. 1 (217)
11 z/h z/h z/h z/h Stresses(Mechanical load, Nx & Mx) on Laminate (a/h=5, [+]as) TaoXY XY Stresses(Mechanical load, Nx & Mx) on Laminate (a/h=5, [+3]as) TaoXY XY Stresses(Mechanical load, Nx & Mx) on Laminate (a/h=5, [+45]as) Tao XY Stresses(Mechanical load, Nx & Mx) on Laminate (a/h=5, [+6]as) Tao XY Fig. 7 Variation of stress with laminate thickness ( z h ) for lamination angle (a) [+ ] as & [+9] as (b) [+3] as (c) [+45] as and (d) [+ 6] as for combined mechanical load (N x = 1 N m, M x = 4 N m and a h = 5) Volume 67, No. 1, (217) 217 SjF STU Bratislava 15
12 z/h z/h z/h z/h Stresses(Thermal load,deltat) on Laminate (a/h=5 & [+]as & [+9]as) Tao XY Stresses(Thermal load,deltat) on Laminate (a/h=5 & [+3]as) Tao XY x Stresses(Thermal load,deltat) on Laminate (a/h=5 & [+45]as) Tao XY Stresses(Thermal load,deltat) on Laminate (a/h=5 & [+6]as) Tao XY Fig. 8 Variation of stress with laminate thickness ( z h ) for lamination angle (a) [+ ] as & [+9] as (b) [+3] as (c) [+45] as and (d) [+ 6] as for thermal load ( T = 75 and a h = 5) SjF STU Bratislava Volume 67, No. 1 (217)
13 z/h z/h z/h z/h Stresses(Thermo Mechanical load, Nx,Mx & deltat) on Laminate (a/h=5 & [+] & [+9]) TaoXY XY Stresses(ThermoMechanical load, Nx,Mx, deltat) on Laminate (a/h=5 & [+3]) TaoXY XY Stresses(Thermo Mechanical load, Nx,Mx & deltat) on Laminate (a/h=5 & [+45]) TaoXY XY Stresses(Thermo Mechanical load, Nx,Mx & deltat) on Laminate (a/h=5 & [+6]) TaoXY XY Fig. 9 Variation of stress with laminate thickness ( z h ) for lamination angle (a) [+ ] as & [+9] as (b) [+3] as (c) [+45] as and (d) [+ 6] as for thermo mechanical load (N x = 1 N m, M x = 4 N m, T = 75 and a h = 5) Volume 67, No. 1, (217) 217 SjF STU Bratislava 17
14 STRESS RATIO STRESS RATIO MECH THERM THERMOMECH [+3] MECH THERM THERMOMECH a/h a/h [+45] MECH THERM THERMOMECH [+6] MECH THERM THERMOMECH a/h a/h Fig. 1 Comparison of the variation of stress ratio () with thickness ratio (a/h) for mechanical, thermal and thermo mechanical load for different lamination angle a/h = 5 a/h = 1 a/h = 2 THERMO MECHANICAL LOAD 1.8 a/h = 5 MECHANICAL LOAD a/h = a/h = LAMINATION ANGLE (DEG) LAMINATION ANGLE(DEG) Fig. 11: variation of stress ratio with lamination angle for different a/h ratio for mechanical and thermo mechanical load SjF STU Bratislava Volume 67, No. 1 (217)
15 STRESS RATIO STRESS RATIO 1.7 MECHANICAL LOAD 1.15 THERMO MECHANICAL LOAD DEG 3 DEG 45 DEG 6 DEG 9 DEG DEG 3 DEG 45 DEG 6 DEG 9 DEG a/h a/h Fig. 12: variation of stress ratio with a/h ratio for different lamination angle for mechanical and thermo mechanical load Mechanical load [+] & [+9] 1.25 Mechanical load [+3] 1.2 a/h = 5 a/h = 1 a/h = a/h = 5 a/h = 1 a/h = NO. OF LAMINA NO. OF LAMINA 1.25 Mechanical load [+6] 1.25 Mechanical load [+45] 1.2 a/h = 5 a/h = 1 a/h = a/h = 5 a/h = 1 a/h = NO. OF LAMINA NO. OF LAMINA Volume 67, No. 1, (217) 217 SjF STU Bratislava 19
16 1.25 Thermo Mechanical load [+] & [+9] [+3] Thermo mechanical load 1.2 a/h = 5 a/h = 1 a/h = a/h = 5 a/h = 1 a/h = NO. OF LAMINA NO. OF LAMINA 1. [+45] Thermo mechanical load 1. [+6] Thermo Mechanical load a/h = 5 a/h = 1 a/h = a/h = 5 a/h = 1 a/h = NO. OF LAMINA NO. OF LAMINA Fig. 13 variation of stress ratio with no. of lamina for different lamination angle for mechanical and thermo mechanical load. 5. Conclusion Composite plate subjected to thermo mechanical load find wide application in aerospace, military, medical, automobile sector etc. This paper present a model to analyze a composite plate subjected to different loading conditions. Classical laminate theory is used to solve the model. It is concluded from the analysis that the optimum lamination angle for combined mechanical load is [+3] and for thermo mechanical load is [+6] at which the stress ratio is minimum. The stress ratio () decreases with the increase in a h ratio and number of lamina. The problem is solved by using both CLT method and FEA.The result of both the method shows good agreement with each other with minor percentage error (3% 5%). Finite element tool (ANSYS) may be a more appropriate method to find the approximate solution to the stress and strain analysis of complex composite plate problem where it is not possible to solve the mathematical model. REFERENCES [1] L.W. Chen, L.Y. Chen. Thermal deformation and stress analysis of composite laminated plates by finite element method, Computers and Structures, Vol. 35, 199 (6), SjF STU Bratislava Volume 67, No. 1 (217)
17 [2] O. Sayman. An elastic plastic thermal stress analysis of aluminium metal matrix composite beams, Composite Structures, 21 (53), [3] O. Ozcan, N. B. Bektas. Elasto plastic stress analysis in simply supported thermo plastic laminated plates under thermal loads, Composite Science and Technology, 21 (61), [4] F. R. Jones, F. Zhao. Thermal loading of short fibre composites and the induction of residual shear stresses, Composites: Part A, 27, [5] C. H. Wu, T. R. Tauchert. Thermoelastic analysis of laminated plates, 1. Symmetric specially orthotropic laminates, Thermal Stresses, 198 (3), [6] A.K. Noor, W.S. Burton, Assessment of shear deformation theories for multilayered composite plates. Applied Mechanics Reviews, 1989, (42), [7] S. Savithri, T. K. Varadan. A Simple Higher Order Theory for Homogeneous Plates. Mechanics: Research Communications, 1992 (19), No. 1, [8] P. Vidal, O. Polit. A thermomechanical finite element for the analysis of rectangular laminated beams. Finite. Elem. Anal. Des., 26 (42), [9] T. B. Zineb et al. Analysis of High Stress Gradients in Composite Plates with Rapidly Varying Thickness. Composites Science and Technology, 1998 (58), [1] M. G. Joshi, S. B. Biggers, Jr. Thickness Optimization for Maximum buckling loads in Composite Laminated plates, Composites: Part B, 1996 (27B), [11] H. Javadi, I. Rajabi, V. Yavari, M. H. Kadivar. Threedimensional solutions for contact area in laminated composite pinned joints with symmetric and nonsymmetric stacking sequences, Journal of Mechanical Engineering Strojnícky časopis, 27 (58), No. 6, [12] E. Kormaníková. Optimal design of laminate circular cylindrical shell 34. Journal of Mechanical Engineering Strojnícky časopis, 27 (58), No. 6, [13] S. S. Choudhary, V.B. Tungikar. A simple higherorder theory for dynamic analysis of composite plate. Journal of Mechanical Engineering Strojnícky časopis, 21 (61), No. 3, [14] Autar K. Kaw, Mechanics of Composite material, second edition, Taylor & Francis, 26. [15] Khoo Ban Han, Fiber reinforced composite laminate plate for varying thickness, Thesis, University of Technology, Malysia Volume 67, No. 1, (217) 217 SjF STU Bratislava 21
18 SjF STU Bratislava Volume 67, No. 1 (217)
Bending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationSound Propagation through Media. Nachiketa Tiwari Indian Institute of Technology Kanpur
Sound Propagation through Media Nachiketa Tiwari Indian Institute of Technology Kanpur LECTURE13 WAVE PROPAGATION IN SOLIDS Longitudinal Vibrations In Thin Plates Unlike 3D solids, thin plates have surfaces
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationDesign of Automobile Driveshaft using Carbon/Epoxy and Kevlar/Epoxy Composites
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp173179 www.ajer.org Research Paper Open Access Design of Automobile Driveshaft using Carbon/Epoxy
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationQuestion 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H
Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationStability Analysis of a Plane, Rectangular, Boron epoxy Laminated Plate Basing on Strength Properties Determined by Different Methods
Mechanics and Mechanical Engineering Vol. 15, No. 2 (2011) 161 181 c Technical University of Lodz Stability Analysis of a Plane, Rectangular, Boron epoxy Laminated Plate Basing on Strength Properties Determined
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMechanics of Solids notes
Mechanics of Solids notes 1 UNIT II Pure Bending Loading restrictions: As we are aware of the fact internal reactions developed on any crosssection of a beam may consists of a resultant normal force,
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationFREE VIBRATION OF THERMALLY PRE/POSTBUCKLED CIRCULAR THIN PLATES EMBEDDED WITH SHAPE MEMORY ALLOY FIBERS
Journal of Thermal Stresses, 33: 79 96, 2010 Copyright Taylor & Francis Group, LLC ISSN: 01495739 print/1521074x online DOI: 10.1080/01495730903409235 FREE VIBRATION OF THERMALLY PRE/POSTBUCKLED CIRCULAR
More informationFREE VIBRATION ANALYSIS OF THIN CYLINDRICAL SHELLS SUBJECTED TO INTERNAL PRESSURE AND FINITE ELEMENT ANALYSIS
FREE VIBRATION ANALYSIS OF THIN CYLINDRICAL SHELLS SUBJECTED TO INTERNAL PRESSURE AND FINITE ELEMENT ANALYSIS J. Kandasamy 1, M. Madhavi 2, N. Haritha 3 1 Corresponding author Department of Mechanical
More informationIraq Ref. & Air. Cond. Dept/ Technical College / Kirkuk
International Journal of Scientific & Engineering Research, Volume 6, Issue 4, April015 1678 Study the Increasing of the Cantilever Plate Stiffness by Using s Jawdat Ali Yakoob Iesam Jondi Hasan Ass.
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationThe stiffness tailoring of megawatt wind turbine
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The stiffness tailoring of megawatt wind turbine To cite this article: Z M Li et al 2013 IOP Conf. Ser.: Mater. Sci. Eng. 52 052008
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationNUMERICAL INVESTIGATION AND STATISTICAL ANALYSIS OF LASER BENDING OF TITANIUM SHEETS
5 th International & 26 th All India Manufacturing Technology, Design and Research Conference (AIMTDR 2014) December 12 th 14 th, 2014, IIT Guwahati, Assam, India NUMERICAL INVESTIGATION AND STATISTICAL
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationBasic concepts to start Mechanics of Materials
Basic concepts to start Mechanics of Materials Georges Cailletaud Centre des Matériaux Ecole des Mines de Paris/CNRS Notations Notations (maths) (1/2) A vector v (element of a vectorial space) can be seen
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationFinite Element Analysis of Piezoelectric Cantilever
Finite Element Analysis of Piezoelectric Cantilever Nitin N More Department of Mechanical Engineering K.L.E S College of Engineering and Technology, Belgaum, Karnataka, India. Abstract Energy (or power)
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationStudying Decreased Methods of Stress Concentration around Holes and Openings of Plate and Shell Structures Body
International Research Journal of Applied and Basic Sciences 01 Available online at www.irjabs.com ISSN 5188X / Vol, 5 (8): 10081015 Science Explorer Publications Studying Decreased Methods of Stress
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationModeling of the Bending Stiffness of a Bimaterial Beam by the Approximation of OneDimensional of Laminated Theory
. FloresDomínguez Int. Journal of Engineering Research and Applications RESEARCH ARTICLE OPEN ACCESS odeling of the Bending Stiffness of a Bimaterial Beam by the Approimation of OneDimensional of Laminated
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationSeismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design
Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design Elmer E. Marx, Alaska Department of Transportation and Public Facilities Michael Keever, California Department
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationSTRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK Md. S. Uddin 1*, E. V. Morozov 1 and K. Shankar 1 1 School of Engineering and Information
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationA Suggested Analytical Solution for Vibration of Honeycombs Sandwich Combined Plate Structure
International Journal of Mechanical & Mechatronics Engineering IJMMEIJENS Vol:16 No:04 9 A Suggested Analytical Solution for Vibration of Honeycombs Sandwich Combined Plate Structure Muhsin J. Jweeg College
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationVIBRATION ENERGY FLOW IN WELDED CONNECTION OF PLATES. 1. Introduction
ARCHIVES OF ACOUSTICS 31, 4 (Supplement), 53 58 (2006) VIBRATION ENERGY FLOW IN WELDED CONNECTION OF PLATES J. CIEŚLIK, W. BOCHNIAK AGH University of Science and Technology Department of Robotics and Mechatronics
More informationFailure interaction curves for combined loading involving torsion, bending, and axial loading
Failure interaction curves for combined loading involving torsion, bending, and axial loading W M Onsongo Many modern concrete structures such as elevated guideways are subjected to combined bending, torsion,
More informationThermoMechanical Response of Functionally Graded Materials for Extreme Environments
ThermoMechanical Response of Functionally Graded Materials for Extreme Environments Introduction In recent years, functionally graded materials (FGMs) have attracted much interest in a wide range of engineering
More informationAPPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS
APPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS L. Zu, S. Koussios and A. Beukers Design and Production of Composite Structures, Faculty of Aerospace Engineering
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationAn Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire. Ziqing Yu¹ and Aixi Zhou²
An Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire Ziqing Yu¹ and Aixi Zhou² ¹Department of Engineering Technology, University of North Carolina at
More informationBE Semester I ( ) Question Bank (MECHANICS OF SOLIDS)
BE Semester I ( ) Question Bank (MECHANICS OF SOLIDS) All questions carry equal marks(10 marks) Q.1 (a) Write the SI units of following quantities and also mention whether it is scalar or vector: (i)
More information